Porous silicon-based nanostructured microparticles as degradable supports for solid-phase synthesis and release of oligonucleotides
© McInnes and Voelcker.; licensee Springer. 2012
Received: 15 May 2012
Accepted: 18 June 2012
Published: 12 July 2012
We describe the preparation of several types of porous silicon (pSi) microparticles as supports for the solid-phase synthesis of oligonucleotides. The first of these supports facilitates oligonucleotide release from the nanostructured support during the oligonucleotide deprotection step, while the second type of support is able to withstand the cleavage and deprotection of the oligonucleotides post synthesis and subsequently dissolve at physiological conditions (pH = 7.4, 37°C), slowly releasing the oligonucleotides. Our approach involves the fabrication of pSi microparticles and their functionalisation via hydrosilylation reactions to generate a dimethoxytrityl-protected alcohol on the pSi surface as an initiation point for the synthesis of short oligonucleotides.
KeywordsPorous silicon Solid-phase DNA synthesis Microparticles
Single-stranded DNA can be produced in a controlled, stepwise manner  using commercial DNA synthesisers on solid supports [1, 2]. Once synthesised, the DNA strand is released from the solid support into solution, deprotected and collected (these three steps are usually carried out in aqueous ammonium hydroxide). Side reactions and failure sequences limit the ultimate length of the oligonucleotides to approximately 100 nucleotides. The oligonucleotides produced in this fashion can be used as antisense strands, small interfering RNA and molecular probes. It is also possible to synthesise RNA, locked nucleic acids and peptide nucleic acids using this methodology.
Controlled pore glass (CPG) is the most common solid support for solid-phase DNA synthesis , although a number of other supports have also been explored including polystyrene [3, 4], carbon [5–7], gold [8, 9], as well as glass and silicon [10–14]. However, due to the insolubility of these supports, mechanical separation is required to harvest the newly synthesised DNA. This separation step can result in reduced yields and increased synthesis times . Thus, efforts to improve the efficiency of DNA synthesis have focused on improving the release of DNA. Some research labs have attempted this by focusing on designing new linkers for use on CPG surfaces [16–18], while other labs have attempted to improve the original nucleoside loading of CPG  or generate new phosphoramidite and solid-phase chemistry . For example, Azhayev  reported on the synthesis of CPG derivatised with long-chain alkyl amino groups, which facilitated faster cleavage of the 3′-terminal phosphodiester group through the action of a secondary hydroxyl group .
DNA synthesis has been attempted on porous silicon (pSi) films as well as single crystalline Si(111) and pSi micro- and nano-particles [21–23] for use in electrochemical sensing applications. The combination of DNA and pSi is of interest to biosensor development due to the unique optical and electrical properties of pSi [24–29]. Most recently, Rea et al.  have demonstrated the synthesis of a ten-base oligonucleotide directly on two different porous silicon-based Bragg reflectors, one oxidised by a thermal treatment, the other by a chemical process based on exposure to I2/pyridine. The synthesis could be monitored by dimethoxytrityl (DMT) release as well as by a red shift in the optical spectra of the Bragg reflector.
However, one of the advantages of pSi, which has so far remained unexplored in the context of solid-phase DNA, is its ability to degrade in aqueous milieu including biological fluids [31, 32], which can be exploited for the on-demand release of the synthesised DNA strands from the surface or for the dissolution of the solid support in situ. pSi undergoes oxidative hydrolysis forming silicic acid (Si(OH)4), which is non-toxic and comprises nearly 95% of naturally occurring silicon in the environment . It is also possible to exploit the electrochemical fabrication processes in order to control the degradation rates, which in turn could control the release of surface-bound oligonucleotides. pSi can be functionalised on either hydride-terminated or hydroxyl-terminated surfaces with relatively mild reaction conditions and widely available chemicals, allowing further control over the degradation rate [34, 35]. Furthermore, pSi can be produced in structures such as microparticles (ranging from tens to hundreds of micrometers). The microparticle size can easily be controlled by the use of sonication  and ball milling [37, 38].
Dichloromethane (CH2Cl2, commercial grade; Merck, North Ryde, Australia) and hexane (commercial grade; Southern Cross, Melbourne, Australia) were distilled over CaH2 and stored over molecular sieves away from light. Tetrahydrofuran and toluene (Aldrich, New South Wales, Australia) were distilled over sodium and benzophenone and stored over molecular sieves away from light. Sodium metal (Riedel-de Haen, Seelze, Germany) was used as received after removal of the paraffin oil with hexane. 4-Dimethylaminopyridine (Aldrich), 4,4′-dimethoxytrityl chloride (Fluka, Buchs, Switzerland) and diethylether (analytical grade; Merck) were used as received. Hydrofluoric acid (Merck), MeOH (Merck), acetone (Ajax, Auburn, Australia) and EtOH (Ajax) were used for etching and washing without further purification. N,N-dimethylformamide (DMF; EMD Chemicals, Billerica, MA, USA) was purified, drying over MgSO4 followed by distillation at reduced pressure . MilliQ water 18.2 MΩ was obtained from a Labconco, Water Pro PS water purifier (Kansas City, MO, USA). Deuterated chloroform (Cambridge Isotope Laboratories, Inc., Andover, MA, USA) was used without further purification. ω-Undecylenyl alcohol (Aldrich) and 10-undecylenic acid were used as received.
Phosphate buffered saline (PBS) was prepared from sodium chloride (NaCl, 8 g L−1; Chemsupply, Port Adelaide, Australia), potassium chloride (KCl, 0.2 g L−1; Biolab Scientific, Scoresby, Australia), di-sodium phosphate di-hydrate (Na2.HPO4.2H2O, 1.12 g L−1; Chemsupply) and potassium dihydrogen orthophosphate (KH2PO4, 0.24 g L−1; Ajax). The pH was adjusted to 7.4 with 1 M NaOH (Ajax) or HCl (Aldrich) in MilliQ water.
Preparation of pSi microparticles
Microparticles were fabricated from p-type Si wafers (boron-doped, resistivity < 0.001 Ω cm, <1-0-0>) supplied by Virginia Semiconductors (Fredericksburg, VA, USA). The wafer was anodised in an 18-cm2 etching cell in 3:1 HF/EtOH solution with a current density of 222 mA cm−2 for 4 min, and then electropolished for 30 s at 500 mA cm−2. CH2Cl2 was then added, and the freestanding porous layer was manually fractured into microparticles for collection. Twenty minutes of sonication in dichloromethane was performed (Soniclean 160HT, 70 W, Soniclean Pty. Ltd., Thebarton, Australia) to transform any large sheets of pSi into smaller particles for recovery. The pSi microparticle suspension was filtered and washed with CH2Cl2 and EtOH. For all subsequent reactions, the pSi microparticle suspension was transferred to a glass reaction vessel containing a fine glass frit (pore size 4.0 to 5.5 μm), and the solvent was removed by aspiration.
pSi microparticles were functionalised via either a cleavable or non-cleavable linker. For full descriptions and schematics of the process, please see Additional file 1. Briefly, fresh pSi microparticles were hydrosilylated with fmoc-11-aminoundecene in mesitylene after deoxygenating with three freeze-pump-thaw cycles. Subsequently, the fmoc-protecting group was removed by shaking with 25% piperidine in DMF before the ring opening of succinic anhydride was performed on the now-exposed surface-bound amines . Following this, any unreacted amines were capped via acylation with acetic anhydride. The carboxy groups introduced by the ring opening of succinic anhydride were then reduced to alcohol groups with the use of LiAlH4. Finally, the freshly generated OH groups were capped with DMT. The final surface was named long-chain alkyl amino pSi (LCAA pSi). The non-cleavable linker was produced in a similar fashion via the hydrosilylation reaction of ω-undecylenyl alcohol followed by DMT capping.
DNA synthesis and characterisation
Two distinct DNA strands were synthesised. For the cleavable linker, a 19mer (3′-CTT GCC GTA GTT CCA CTT G-5′) was synthesised, and for the non-cleavable linker, a 10mer (3′-CTT GCC GTA G-5′) was used.
All DNA synthesis was performed with UltraMild DNA bases purchased from Glen Research (Sterling, VA, USA), and subsequently, DNA deprotection was performed by incubating the pSi microparticles with either potassium carbonate (0.05 M) in MeOH at room temperature for 4 h or ammonium hydroxide at 60°C overnight. Ammonium hydroxide deprotection can be used for both standard phosphoramidites and the UltraMild DNA bases and is the standard protocol for DNA synthesis. The ammonium hydroxide deprotection was used with the cleavable chemistries as the dissolution of the pSi support was desirable and was 100% complete at the conditions used. For the non-cleavable chemistry presented in this manuscript, the mild deprotection with potassium is preferred to conventional ammonium hydroxide as it facilitates the deprotection of the DNA synthesised with UltraMild bases while allowing the DNA to remain bound to the surface (uncleaved) and the pSi to remain intact (undissolved) for subsequent drug release experiments.
DNA release via UV–vis spectroscopy
UV-visible (UV–vis) spectroscopy was performed on an Agilent 8453 UV–vis spectrophotometer (Agilent Technologies, Santa Clara, CA, USA) using UV-Visible ChemStation Software Rev B.01.01  at a wavelength of 260 nm. Release rates were calculated from the slope of release curves obtained. The actual amount of DNA released was calculated via the use of the Beer-Lambert Law, using the molar extinction coefficient of 194,300 and 90,165 L mol−1 cm−1 for the 19mer and 10mer, respectively. Molar extinction coefficients were calculated from the nearest-neighbour model at 260 nm using previously reported parameters [40, 41]. The amount of DNA released was normalised to the mass of the sample used and then converted to a percentage of the total theoretical payload.
Ziptip extraction and MALDI-MS analysis
DNA release solutions were purified using 10-μL ZiptipC18 pipette tips (Merck Millipore, Billerica, MA, USA). The Ziptips were used according to the manufacturer's protocol. Matrix-assisted laser desorption/ionisation mass spectrometery (MALDI-MS) analysis on the Ziptip-purified DNA was performed on a Waters Micromass M@LDI L/R TOF-MS (Waters Corporation, Milford, MA, USA). The acquisition software was MassLynx 4.1. Analysis was performed in linear mode with the following conditions: polarity, positive ion; source voltage, 15,000 V; pulse voltage, 1,500 V; MCP detector voltage, 1,900 V; laser energy, 89%; matrix suppression, 800 amu; TLF delay, 500.0 ns; and mass range, 1,300 to 15,000 Da.
Infrared (IR) spectra were obtained using a Nicolet Avatar 370MCT (Thermo Electron Corporation, Waltham, MA, USA) equipped with a standard transmission accessory. Spectra were recorded and analysed using OMNIC version 7.0 software in the range of 650 to 4,000 cm−1 at a resolution of 4 cm−1; the background was taken using a blank KBr disc. IR of pSi microparticles was performed with crushed particles (approximately 2 mg) dispersed in KBr discs. The KBr was supplied by Spectra-Tech (Oak Ridge, TN, USA) and was 99.9 + % FT-IR grade. All IR spectra were collected in transmission mode and subsequently converted to absorbance using OMNIC version 7.0 software. All spectra were normalised using the Si-O peak at approximately 1,100 cm−1 and scaling the entire spectra so that the Si-O peak is equal to 1 AU.
Scanning electron microscopy
Scanning electron microscopy (SEM) was performed on a XL30 field emission SEM (Philips, Amsterdam, Netherlands) at an acceleration voltage of 10 keV. pSi microparticles were dispersed directly onto conductive aluminium stubs for analysis.
Results and discussion
Cleavable linker chemistry (LCAA) on pSi microparticles
After fmoc deprotection and ring opening of succinic anhydride, the spectra (Figure 4B) still showed the characteristic peaks listed above and new peaks at 1,695 and 2,237 cm−1, which were attributed to the new C = O vibrations of the succinic anhydride and possibly by Si-H stretching in O3-SiH groups . The IR spectrum of the acetyl-capped and reduced (with LiAlH4) surface can be seen in Figure 4C. The only change was the slight decrease of the peak at 1,695 cm−1 due to the removal of the carbonyl vibration in the terminal carboxylic acid. The final DMT-capped surface (Figure 4D) showed sharper peaks at 1,382 and 1,446 cm−1 as assigned to CH3 umbrella deformation and CH2 deformation, respectively. Additionally, the reappearance of the peak at 673 cm−1 is indicative of C-H out-of-plane deformation vibrations from the benzene. These spectra confirm the presence of the LCAA linker on the surface of pSi.
In order to determine the amount of pSi support required for a standard 40-nmol scale solid-phase DNA synthesis, a pre-weighed amount of the LCAA-functionalised pSi support was reacted with trichloroacetic acid. The thus-generated DMT cation in the supernatant was assayed via UV–vis spectroscopy, and the loading achieved was found to be 13.2 ± 0.3 nmol mg−1 of pSi particles, comparable with the loading levels of conventional CPG (15.0 nmol mg−1 of resin).
The effect of changing synthesis conditions in terms of coupling, detritylation, oxidation and capping steps during automated DNA synthesis of 19mer (3′-CTTGCCGTAGTTCCACTTG-5′) on LCAA-functionalised pSi particles was investigated to determine optimal DNA synthesis conditions onto LCAA-modified pSi. This investigation was carried out since the OY under standard synthesis parameters was relatively low (41.4%). No significant improvements in OY were seen with extended wait times, doubling the volumes of reagents or both simultaneously. However, doubling of coupling time and volume resulted in a significant improvement, resulting in an OY of 76.6%. The improved yield is possibly attributed to the mass transport limitations experienced on the highly porous material at the standard coupling time and concentration. To confirm this observed increased overall yield, duplicate synthesis was performed with the same parameters, and this synthesis resulted in a final OY of 77.3%, demonstrating a reproducibly high yield. This yield compares well with typical yields seen when short oligonucleotides are synthesised on standard CPG (ca. 75% assuming a 99% average stepwise yield) .
To facilitate the slow release of the full-length DNA from the pSi supports post DNA deprotection, a non-cleavable linker was explored for solid-phase DNA synthesis. This linker was designed to be non-cleavable during the DNA deprotection step and facilitate the release of fully deprotected DNA from the pSi scaffold. The linker was introduced by hydrosilylation with ω-undecylenyl alcohol. The functionalised pSi (Figure 6A) shows significant peaks at 1,360 and 1,440 cm−1 and a triple peak at 2,800 to 3,000 cm−1 for C-H vibrations. A strong, broad peak centred at 1,060 cm−1 due to asymmetric stretching vibrations of Si-O-Si surface bridging groups , as well as peaks at 2,060 cm−1 due to the residual Si-H bonds remaining after the hydrosilylation reaction, was also observed. After capping with DMT, the pSi surface (Figure 6B) shows new peaks at 1,250 cm−1 for C-O-C ether stretching and 1,490 cm−1 which corresponds to = C-H and C = C in ring stretching vibrations of benzene rings, demonstrating successful introduction of the protecting group. Alternatively, we were able to introduce the same linker by hydrosilylation of 10-undecylenic acid, followed by reduction with LiAlH4 and DMT capping (results not shown).
DMT loading on the pSi microparticles functionalised with the non-cleavable linker was very good, almost four times higher than for standard CPG and the LCAA-functionalised pSi microparticles (56.9 ± 7.4 nmol mg−1 compared to 15 nmol mg−1).
The synthesis of a 10mer (3′-CTTGCCGTAG-5′) was subsequently performed under optimised solid-phase synthesis conditions. A yield of 66.1% (37.58 nmol of DNA) was obtained, which was only slightly lower than the yield of 10mer for the standard CPG (73.4%).
pSi microparticles functionalised with a 10mer DNA strand and deprotected with 0.05 M potassium carbonate in MeOH retained deprotected DNA on the microparticles, judging from the absence of significant absorbance at 260 nm in the deprotection solution. In contrast, the microparticles functionalised with LCAA chemistry released significant amounts of DNA upon deprotection. The microparticles carrying deprotected DNA were then placed into neutral PBS at 37°C, and DNA release was investigated via measuring the UV–vis absorbance at 260 nm.
We have described the fabrication of pSi-based supports with both cleavable and non-cleavable chemistries for the solid-phase synthesis of DNA on conventional DNA synthesisers with established reagents and protocols. The cleavable LCAA linker was able to withstand the DNA synthesis protocol with similar OYs to CPG, as well as release 99% of fully deprotected synthesised DNA upon treatment with aqueous ammonium hydroxide solution overnight. The simultaneous dissolution of the solid support is also advantageous as it alleviates the need for a filtration step before purification of the DNA. In contrast, pSi surfaces functionalised with the non-cleavable linker were able to retain the synthesised DNA upon deprotection of the nucleobases, and subsequently released a large amount (4.3 nmol mg−1 of pSi) of fully deprotected DNA into PBS at 37°C over 20 h.
The ability to synthesise specific DNA strands on a biodegradable and biocompatible support such as pSi will allow improved control over degradation and drug release profiles. These systems, when combined with a targeting agent, may also be beneficial for the preparation of advanced bio-devices capable of delivering payloads of therapeutic DNA in applications such as gene therapy.
This work was funded by Flinders University and the Australian Research Council.
- Efcavitch J: Automated system for the optimized chemical synthesis of oligodeoxyribosenucleotides. In Macromolecular Sequencing and Synthesis: Selected Methods and Applications, New York: Alan R. Liss, Inc; 1988:221–234.
- Applied B: Section 6: chemistry for automated DNA synthesis. In Applied Biosystems 391 DNA Synthesiser PCR Mate EP User's Guide. Mulgrave: Applied Biosystems 1989, 6: 1–6.
- Ghosh D, Faure N, Kundu S, Rondelez F, Chatterji D: Hybridization and immobilization of long ds-DNAs on polystyrene microspheres. Langmuir 2003, 19(14):5830–5837. 10.1021/la0341963View Article
- Zammatteo N, Girardeaux C, Delforge D, Pireaux J, Remacle J: Amination of polystyrene microwells: application to the covalent grafting of DNA probes for hybridization assays. Anal Biochem 1996, 236(1):85–94. 10.1006/abio.1996.0135View Article
- Millan K, Mikkelsen S: Sequence-selective biosensor for DNA based on electroactive hybridization indicators. Anal Chem 1993, 65: 2317–2323. 10.1021/ac00065a025View Article
- Millan K, Saraullo A, Mikkelsen S: Voltammetric DNA biosensor for cystic fibrosis based on a modified carbon paste electrode. Anal Chem 1994, 66: 2943–2948. 10.1021/ac00090a023View Article
- Wang J, Fernandes J, Kubota L: Polishable and renewable DNA hybridization biosensors. Anal Chem 1998, 70(17):3699–3702. 10.1021/ac980092zView Article
- Frutos A, Liu Q, Thiel A, Sanner A, Condon A, Smith L, Corn R: Demonstration of a word design strategy for DNA computing on surfaces. Nucleic Acids Res 1997, 25(23):4748–4757. 10.1093/nar/25.23.4748View Article
- Frutos A, Smith L, Corn R: Enzymatic ligation reactions of DNA “words” on surfaces for DNA computing. J Am Chem Soc 1998, 120(40):10277–10282. 10.1021/ja982030wView Article
- Chrisey L, Lee G, O'Ferrall C: Covalent attachment of synthetic DNA to self-assembled monolayer films. Nucleic Acids Res 1996, 24(15):3031–3039. 10.1093/nar/24.15.3031View Article
- Lamture J, Beattie K, Burke B, Eggers M, Ehrlich D, Fowler R, Hollis M, Kosicki B, Reich R, Smith S, Varma R, Hogan M: Direct detection of nucleic acid hybridization on the surface of a charge coupled device. Nucleic Acids Res 1994, 22(1):2121–2125. 10.1093/nar/22.11.2121View Article
- Piunno P, Krulla U, Hudson RH, Damhac M, Cohend H: Fiber optic biosensor for fluorimetric detection of DNA hybridization. Anal Chim Acta 1994, 288(3):205–214. 10.1016/0003-2670(93)E0611-AView Article
- Rogers Y, Jiang-Baucom P, Huang Z, Bogdanov V, Anderson S, Boyce-Jacino M: Immobilization of oligonucleotides onto a glass support via disulfide bonds: a method for preparation of DNA microarrays. Anal Biochem 1999, 266(1):23–30. 10.1006/abio.1998.2857View Article
- Souteyrand E, Cloarec J, Martin J, Wilson C, Lawrence I, Mikkelsen S, Lawrence M: Direct detection of the hybridization of synthetic homo-oligomer DNA sequences by field effect. J Phys Chem B 1997, 101: 2980–2985. 10.1021/jp963056hView Article
- Azhayev A, Antopolsky M: Amide group assisted 3′-dephosphorylation of oligonucleotides synthesised on universal A-supports. Tetrahedron 2001, 57: 4977–4986. 10.1016/S0040-4020(01)00409-4View Article
- Laurent A, de Lambert B, Charreyre M, Mandrand B, Chaix C: A one step derivatisation of controlled pore glass for oligonucleotide solid-phase synthesis. Tetrahedron Lett 2004, 45: 8883–8887. 10.1016/j.tetlet.2004.09.167View Article
- Mahajan S, Patnaik S, Gandhi R, Gupta K, Kumar P: Synthesis of labeled oligonucleotides through a new chemically cleavable linker. Tetrahedron Lett 2005, 46: 6149–6153. 10.1016/j.tetlet.2005.06.164View Article
- Pon R, Yu S: Hydroquinone-O, O’-diacetic acid as a more labile replacement for succinic acid linkers in solid phase oligonucleotide synthesis. Tetrahedron Lett 1997, 38(19):3327–3330. 10.1016/S0040-4039(97)00619-9View Article
- Padmanabhan S, Coughlin J, Iyer R: Microwave-assisted functionalisation of solid supports: application in the rapid loading of nucleosides on controlled-pore-glass (CPG). Tetrahedron Lett 2005, 46: 343–347. 10.1016/j.tetlet.2004.09.189View Article
- Dioubankova N, Malakov A, Stetsenko D, Gait M, Korshun V: Phosphoramidites and solid supports based on N-substituted 2,4-dihydroxybutyramides: universal reagents for synthesis of modified oligonucleotides. Tetrahedron 2006, 62: 6762–6773. 10.1016/j.tet.2006.05.008View Article
- Bessueille F, Dugas V, Vikulov V, Cloarec J, Souteyrand E, Martin J: Assessment of porous silicon substrate for well-characterised sensitive DNA chip implement. Biosens Bioelectron 2005, 21: 908–916. 10.1016/j.bios.2005.02.007View Article
- Lie L, Patole S, Pike A, Ryder L, Connolly B, Ward A, Tuite E, Houlton A, Horrocks B: Immobilisation and synthesis of DNA on Si(111), nanocrystalline porous silicon and silicon nanoparticles. Faraday Discuss 2004, 125: 235–249.View Article
- Pike A, Lie L, Eagling R, Ryder L, Patole S, Connolly B, Horrocks B, Houlton A: DNA on silicon devices: on-chip synthesis, hybridisation, and charge transfer. Angew Chem Int Ed 2002, 41(4):615–617. 10.1002/1521-3773(20020215)41:4<615::AID-ANIE615>3.0.CO;2-YView Article
- Janshoff A, Dancil K, Steinem C, Greiner D, Lin V, Gurtner C, Motesharei K, Sailor M, Ghadiri M: Macroporous p-type silicon Fabry-Perot layers: fabrication, characterization, and applications in biosensing. J Am Chem Soc 1998, 120(46):12108–12116. 10.1021/ja9826237View Article
- Thust M, Schoening M, Frohnhoff S, Arens-Fischer R, Kordos P, Lueth H: Porous silicon as a substrate material for potentiometric biosensors. Meas Sci Technol 1996, 7(1):26–29. 10.1088/0957-0233/7/1/003View Article
- Archer M, Christophersen M, Fauchet P: Macroporous silicon electrical sensor for DNA hybridization detection. Biomed Microdevices 2004, 6(3):203–211.View Article
- Schoning M, Kurowski A, Thust M, Kordos P, Schultze J, Luth H: Capacitive microsensors for biochemical sensing based on porous silicon technology. Sensor Actuat B-Chem 2000, 64(1–3):59.View Article
- Bayliss S, Hutt D, Zhang Q, Harris P, Phillips N, Smith A: Structural study of porous silicon. Thin Solid Films 1995, 255(1–2):128.View Article
- Pividori M, Merkoci A, Alegret S: Electrochemical genosensor design: immobilisation of oligonucleotides onto transducer surfaces and detection methods. Biosens Bioelectron 2000, 15(5–6):291.View Article
- Rea I, Oliviero G, Amato J, Borbone N, Piccialli G, Rendina I, Stefano LD: Direct synthesis of oligonucleotides on nanostructured silica multilayers. J Phys Chem C 2010, 114: 2617–2621. 10.1021/jp908440uView Article
- Anderson S, Elliott H, Wallis D, Canham L, Powell J: Dissolution of different forms of partially porous silicon wafers under simulated physiological conditions. Phys Status Solidi A 2003, 197: 331–335. 10.1002/pssa.200306519View Article
- Canham L: Bioactive silicon structure fabrication through nanoetching techniques. Adv Mater 1995, 7(12):1033–1037. 10.1002/adma.19950071215View Article
- Canham L, Aston R: Will a chip everyday keep the doctor away? Phys World 2001, 27: 31.
- McInnes SJP, Voelcker NH: Silicon-polymer hybrid materials for drug delivery. Future Med Chem 2009, 1(6):1051–1074. 10.4155/fmc.09.90View Article
- Schmeltzer J, Buriak J In The chemistry of nanomaterials: Synthesis, properties and applications. In Recent developments in the chemistry and chemical applications of porous silicon. Rao C, Muller A, Cheetham A. Weinheim, Wiley-VCH; 2004.View Article
- Cunin F, Schmedake T, Link J, Li Y, Koh J, Bhatia S, Sailor M: Biomolecular screening with encoded porous-silicon photonic crystals. Nat Mater 2002, 1: 39–41. 10.1038/nmat702View Article
- Donato MG, Monaca MA, Faggio G, Stefano LD, Jones PH, Gucciardi PG, Marago OM: Optical trapping of porous silicon nanoparticles. Nanotechnology 2011, 22(50):505704/1–505704/8.View Article
- Russo L, Colangelo F, Cioffi R, Rea I, Stefano LD: A mechanochemical approach to porous silicon nanoparticles fabrication. Materials 2011, 4: 1023–1033. 10.3390/ma4061023View Article
- Armarego W, Perrin D: Purification of Laboratory Chemicals. 4th edition. Butterworth-Heinemann, Oxford; 1996.
- Cantor CR, Warshaw MM, Shapiro H: Oligonucleotide interactions. III: circular dichroism studies of the conformation of deoxyoligonucleotides. Biopoly 1970, 9: 1059–1077. 10.1002/bip.1970.360090909View Article
- Handbook of Biochemistry and Molecular Biology, volume 1: Nucleic acids: CRC Press. G.D. Fasman, CRC Press; 1975:589.
- Halimaoui A: In Properties of porous silicon. Short Run Press, Edited by Canham L. London; 1997.
- Bisi O, Ossicini S, Pavesi L: Porous silicon: a quantum sponge structure for silicon based optoelectronics. Surf Sci Rep 2000, 38: 1–126. 10.1016/S0167-5729(99)00012-6View Article
- Mirji SA, Halligudi SB, Mathew N, Ravia V, Jacob NE, Patil KR: Adsorption of methanol on Si(100)/SiO2 and mesoporous SBA-15. Colloids Surf, A 2006, 287: 51–58. 10.1016/j.colsurfa.2006.03.021View Article
- Boukherroub R, Wayner D, Sproule G, Lockwood D, Canham L: Stability enhancement of partially-oxidized porous silicon nanostructures modified with ethyl undecylenate. Nano Lett 2001, 1(12):713–717. 10.1021/nl010061aView Article
- Giovannozzia AM, Rocchia M: Effect of the reaction time, reagent concentration and sample thickness on the thermal derivatisation of p + porous silicon with α-undecene and ω-carboxy alkenes: a FTIR investigation. Sens Actuators B 2008, 130(2):795–801. 10.1016/j.snb.2007.10.043View Article
- Sweetman MJ, Harding FJ, Graney SD, Voelcker NH: Effect of oligoethylene glycol moieties in porous silicon surface functionalisation on protein adsorption and cell attachment. Appl Surf Sci 2011, 257(15):6768–6774. 10.1016/j.apsusc.2011.02.122View Article
- Larson RA, Weber EJ: Reaction Mechanisms in Environmental Organic Chemistry. Lewis Publishers, New York; 1994.
- Wu E, Park J-H, Park J, Segal E, Cunin F, Sailor M: Oxidation-triggered release of fluorescent molecules or drugs from mesoporous Si microparticles. ACS Nano 2008, 2(11):2401–2409. 10.1021/nn800592qView Article
- Ruminski AM, King BH, Salonen J, Snyder JL, Sailor MJ: Porous silicon-based optical microsensors for volatile organic analytes: effect of surface chemistry on stability and specificity. Adv Funct Mater 2010, 20: 2874–2883. 10.1002/adfm.201000575View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.